Structures and Phase Transitions of the <i>A</i>~7~PSe~6~ (<i>A</i> = Ag, Cu) Argyrodite-Type Ionic Conductors. I. Ag~7~PSe~6~
Evain, M.; Gaudin, E.; Boucher, F.; Petricek, V.; Taulelle, F.; Acta Crystallographica Section B 54 (1998) 376–383; doi:10.1107/S0108768197019654

data_2003006
_publ_section_title
;
 Structures and Phase Transitions of the <i>A</i>~7~PSe~6~ (<i>A</i> =
 Ag, Cu) Argyrodite-Type Ionic Conductors. I. Ag~7~PSe~6~
;
_journal_issue                   4
_journal_name_full               'Acta Crystallographica Section B'
_journal_page_first              376
_journal_page_last               383
_journal_paper_doi               10.1107/S0108768197019654
_journal_volume                  54
_journal_year                    1998
_chemical_formula_moiety         'Ag7 P Se6'
_chemical_formula_sum            'Ag7 P Se6'
_chemical_formula_weight         1259.8
_space_group_crystal_system      cubic
_space_group_IT_number           216
_space_group_name_Hall           'F -4 2 3'
_space_group_name_H-M_alt        'F -4 3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   10.838(3)
_cell_length_b                   10.838(3)
_cell_length_c                   10.838(3)
_cell_measurement_reflns_used    26
_cell_measurement_temperature    473
_cell_volume                     1273.1(6)
_diffrn_ambient_temperature      473
_diffrn_measurement_device       'Siemens P4'
_diffrn_measurement_method       \w
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_type           'Ag K-L~2,3~'
_diffrn_radiation_wavelength     .56090
_diffrn_reflns_av_R_equivalents  .056
_diffrn_reflns_limit_h_max       18
_diffrn_reflns_limit_h_min       0
_diffrn_reflns_limit_k_max       18
_diffrn_reflns_limit_k_min       0
_diffrn_reflns_limit_l_max       18
_diffrn_reflns_limit_l_min       0
_diffrn_reflns_number            2513
_diffrn_reflns_theta_max         50
_diffrn_reflns_theta_min         0
_diffrn_standards_decay_%        <1
_diffrn_standards_interval_count 100
_diffrn_standards_number         3
_exptl_absorpt_coefficient_mu    14.65
_exptl_absorpt_correction_T_max  .285
_exptl_absorpt_correction_T_min  .271
_exptl_absorpt_correction_type   sphere
_exptl_crystal_colour            'metallic luster'
_exptl_crystal_density_diffrn    6.569
_exptl_crystal_density_meas      ?
_exptl_crystal_description       sphere
_exptl_crystal_F_000             2192
_refine_diff_density_max         .67
_refine_diff_density_min         -.74
_refine_ls_extinction_coef       .22(3)
_refine_ls_extinction_method
; Isotropic secondary extinction - Type I - Gaussian distribution (Becker
& Coppens, 1974)
;
_refine_ls_goodness_of_fit_obs   1.40
_refine_ls_matrix_type           fullcycle
_refine_ls_number_parameters     33
_refine_ls_number_reflns         192
_refine_ls_number_restraints     0
_refine_ls_R_factor_obs          .0326
_refine_ls_shift/esd_max         <0.0001
_refine_ls_structure_factor_coef F
_refine_ls_weighting_details     w=1/[\s^2^(Fo)+(0.018Fo)^2^]
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_obs         .0372
_reflns_number_observed          1116
_reflns_number_total             248
_reflns_observed_criterion       >3sigma(I)
_cod_data_source_file            lc0002.cif
_cod_data_source_block           gammaAg7
_cod_depositor_comments
;
 Changing the space group from 'P -4 2 3' to 'F -4 2 3' after consulting
 the original publication. All related space group information was changed
 accordingly.

 Antanas Vaitkus,
 2017-07-04

The following automatic conversions were performed:

'_exptl_absorpt_correction_type' tag value 'spherical' was replaced
with 'sphere' value.

Automatic conversion script
Id: cif_fix_values 1646 2011-03-28 12:23:43Z adriana 

The following automatic conversions were performed:

'_refine_ls_weighting_scheme' value 'calc
w=1/[\s^2^(Fo)+(0.018Fo)^2^]' was changed to 'calc'. New tag
'_refine_ls_weighting_details' was created. The value of the new tag
was set to 'w=1/[\s^2^(Fo)+(0.018Fo)^2^]'.

Automatic conversion script
Id: cif_fix_values 3143 2015-03-26 13:38:13Z robertas 
;
_cod_original_cell_volume        1273.1(12)
_cod_database_code               2003006